MODELING OF 3M VHB ADHESIVE TAPE FOR GLAZING SYSTEM ASSEMBLY Fay Salmon, Ph.D. Senior Research Specialist 3M St. Paul, MN
Fay Salmon is a Senior Research Specialist at the SEMS Corporate Research Lab of 3M. She holds a Ph.D. in Mechanical Engineering. Her primary job functions include supporting 3M technology and product development through structural analysis, material characterizations, and modeling and simulation. Prior to her current position, she was an assistant professor at Tennessee Tech University, then as a research engineer at Third Wave Systems developing simulation software for metal machining. She is a member of ASME and ASM International.
MODELING OF VHB STRUCTURAL GLAZING TAPE FOR GLAZING SYSTEM ASSEMBLY
Fay Salmon, Senior Research Specialist, 3M Company, St. Paul, MN Qihong Nie, Structural Analyst, 3M Company, St. Paul, MN Steve Austin, Global Technical Service Specialist, 3M Company, St. Paul, MN Brent Bystrom, Technical Service Specialist, 3M Company, St. Paul, MN February 28, 2013 Abstract This work demonstrated a process to evaluate the long-term performance of VHB Structural Glazing Tape G23F (VHB G23F) in applications where the glass panels have initial warpage. Glazing panel structures bonded with VHB acrylic foam adhesive tapes were analyzed to evaluate the warpage tolerance and the long term strength of the bond when the panels are not flat upon assembly. To simulate VHB adhesive tapes that exhibit nonlinear elastic and viscoelastic behavior, time- and temperature-dependent material models were developed and incorporated into finite element analysis. Simulations were performed to determine first, the contact pressure at the interface of the adhesive tape and glass panel during the bond assembly process, then the residual stress in the adhesive tape due to spring-back of warped glass panels after the bonding pressure was removed. Based on the residual stress and creep rupture strength data developed in previous work, the long-term bond strength was evaluated. The analysis results indicate that the VHB adhesive bond can accommodate a certain amount of warpage of the glazing panel due to the combination of the adhesives bond strength and its hyperelastic-viscoelastic properties that enable stress relaxation and reduction of spring-back stress. The results also showed the effect of the warpage on the wet-out pressure and residual stress due to spring-back of the initially warped glass.
Key words: VHB G23F, adhesive modeling, glazing panel, deformation tolerance, hyperelastic material, viscoelastic material Introduction High performance pressure-sensitive adhesive (PSA) tapes, such as VHB Structural Glazing Tape G23F (VHB G23F), have been increasingly used to attach glass panels to structural glazing frames replacing dry-glazed (gasket, mechanical fasteners, pressure plate, etc.) or wet-glazed (structural silicone sealants) systems. The VHB G23F glazing adhesive is a PSA tape with an adhesive foam core that provides extra compliance when bonding two relatively rigid substrates. This tape is a closed cell, double-sided acrylic foam tape that has the capability to develop very high bond strength. Compared with the traditional bonding material of structural silicone sealants, the VHB G23F tape offers immediate handling strength, consistent bond quality due to ease of application in the bonding process, tolerance to thermal mechanical stresses, as well as long-term strength, durability, weatherability, and UV resistance.
Traditionally, in a structurally glazed system the weight of the glass panel is supported mechanically along the lower horizontal supporting fin or fixture, while the live wind load and thermal mechanical load due to thermal expansion mismatch of the components in glazing structures are supported mainly by the adhesive bond. To ensure long-term performance, high bond quality needs to be established in the glazing assembly process. This can become less certain when the glass panels to be bonded are not flat. Various distortions such as overall bow, warp, and roller wave may be present in glass panels as a result of heat treatment, particularly tempering and heat strengthening processes. ASTM Standard C 1048, Standard Specification for Heat-Strengthened and Fully Tempered Flat Glass provides the specification for allowable warpage for glass panels. Structural silicone sealants are gap-filling, conformable, and flowable before curing, which allow them to accommodate initial warpage of the glass panels. VHB G23F tape is a fully cured adhesive with a predefined thickness and width, and as such, has limited gap-filling capabilities. When the glass panels are warped, bonding the panels to the rigid structural frame requires sufficient bonding pressure to achieve wet-out (contact) at the bonding interface to form the bond. In addition, residual stresses may develop at the bond line when the warped glass springs back after the assembly pressure is removed which, over time, may lead to bond failure in the warped areas if the residual stresses are sufficiently high. The focus of this paper is, therefore, to develop a process to effectively evaluate the wet-out pressure, the residual stresses, and the long term bond strength when glass panels are not flat. This is achieved by first developing adhesive material models to enable the simulation of an adhesive tape, VHB G23F, during a glazing assembly process. The wet-out pressure and residual stresses are then investigated through modeling. Finally, the long term durability of the bond is evaluated following the framework developed in a previous study of Townsend, et al. [1, 2, and 3] that employs the creep rupture strength of this adhesive tape. This previous work will be reviewed in the following section to provide background information. Other studies in the area of adhesive bond joint strength measurements and evaluation for construction applications can be found in the experimental work of Turner, et al.  which demonstrated that the addition of construction adhesive of polyurethane improved joint performance to resist uplift wind forces at the roof framing connection. The study of Jacobs, et al.  measured the improvement of wood roof structural joints under monotonic load condition when acrylic foam adhesive tapes are introduced to the joint. Further analysis of the bonded joint strength was not performed in these two studies. Previous Work on VHB G23F Adhesive Tape The durability of VHB G23F tape, the structural glazing adhesive tape manufactured by 3M, and its application to window glazing have been investigated by Townsend, et al. in an earlier work presented in multiple publications [1, 2, and 3]. In this early work, a large and statistically significant body of both adhesive constitutive material property data and creep rupture strength data were generated for the VHB G23F tape bonded to anodized aluminum substrates.
First, their experimental measurements of VHB G23F tapes tensile, shear, and through-the-thickness material properties produced a set of consistent time-temperature superposition shift factors, aT, that could be modeled accurately using the Williams-Landel-Ferry (WLF) equation. The measured WLF constants were reported as C1 = 9.98 and C2 = 132.6C at a reference temperature of 30C. Furthermore, they demonstrated that the shift factors generated from the dynamic mechanical analyzer (DMA) test can be applied to shift creep rupture strength data of the same tape into smooth master curves, making the construction of such master curves at the long time duration range possible by applying the time-temperature superposition principle (TTSP) using the shift factors from DMA tests. This master curve of creep rupture time (time to failure) for the VHB G23F tape is replicated here in Fig. 1. To make it easier to use in evaluation of creep rupture time, the master curve was fitted by a power law [2, 3] as follows: = ( ) = 0.01724 . (1)
where, = tensile stress on the adhesive tape (MPa)
ft = time to failure (seconds) and the equation is for a reference temperature of 30C .
Figure 1. Tensile stress rupture time master curve of the VHB G23F tape from Townsend, et al. [1, 2 and 3].
10^1 10^2 10^3 10^4 10^5 10^6 10^7 10^8
Failure time (seconds)
Shifted Tensile 23 C, log(aT) = 0.575
Shifted Tensile 40 C, log(aT) = -0.720
Shifted Tensile 60 C, log(aT) = -1.825
Regression Fit, (Stress, MPa) = 0.6049(Time, sec.)^-0.1238
Reference Temperature: 30oCPoints are average of nine replicatesFit of replicate averages to regression line: R2 = 0.97
To assess the effect of the dynamic cyclic wind load on the bonds long term durability, Townsend, et. al. [2, 3] postulated that the Palmgren-Miner linear damage accumulation model is applicable to evaluate the VHB G23F bond strength: = , (2)
where, Ld = the length of time encompassed by a wind history, Ls = the desired service life, n = the number of entries in the wind load history, ti = the time duration of the ith wind load entry from the wind history, tfail,i = the stress rupture time of the ith wind load entry, n = number of wind load entry. This model then predicts that failure occurs when the damage sums to unity, or D = 1. To use this model, Townsend, et al. suggested that the stress rupture time of the ith wind load entry, tfail,i, in Eq. 2 could be evaluated from the master curve of the creep rupture time (Eq. 1). One requirement for this model to be applicable is that the failure mode of the bond has to be the same at all the stress levels within the range of this master curve. The experiments in Townsends work [1, 2] showed that when the specimens were tested at lower stresses for longer duration, the failed specimens exhibited a combination of cohesive and adhesive failure surfaces, while in the higher-stress and shorter-duration tests, specimens exhibited a primarily cohesive failure mode. This tends to suggest that one implicit assumption when applying this master curve for bond strength evaluation is that the bond failure mode is cohesive, not adhesive, for all the time durations. This assumption is further supported by field evaluations of real glazing structures for more than 20 years which showed no evidence of adhesive failure . Therefore this assumption can be considered reasonable. Due to the long-term nature of the creep and relaxation failure, limited experimental data are available to validate the models proposed by Townsend, et al. described above, especially for failure times greater than 20 to 50 years. However, the work of Townsend, et al. presents a simple approach and relatively compelling arguments based on the most extensive experimental data yet generated for the VHB G23F tape. As mentioned earlier, field data accumulated from various projects over more than 20 years support the observations of their test data, even though carefully controlled laboratory experimental data are still limited. Therefore, this current work will follow the same framework and use their creep rupture master curves to evaluate the long term bond strength of the same adhesive tape. As the experimental measurement capabilities continue to develop and more material data are generated, better understanding is expected in the future.
Glazing Panel Assembly The glazing panel assembly process is described here briefly to illustrate the model and steps used in the finite element analyses performed in this work. Typically the window glazing structures are assembled off-site at a glazing facility. Fig. 2 illustrates a simplified window glazing assembly. A typical assembly process involves multiple steps, including the following:
1. VHB G23F tape is applied first to the aluminum glazing frame followed by initial pressure applications to facilitate contact or wet-out to the aluminum frame.
2. A glass panel, which may have a slight warpage, is placed, in the horizontal position, over the exposed tape as illustrated in Fig. 2. The weight of the glass panel will cause initial contact with the tape; however, the warped area of the glass panel may not make contact with the tape (warpage of the glass panel is greatly exaggerated in Fig. 2 to better illustrate the warped panel concept).
3. A bond is formed by applying pressure along the edges of the glass panel over the area where the adhesive tape is located. Typically this is done by a mechanically-driven pressure roller that applies a force of 222 N (50 lb) and rolls around the entire perimeter of the glass panel, forcing the glass to make contact with the VHB G23F tape.
4. Once the bond is formed, the bonding pressure is removed and the warped glass is allowed to spring back while the edges are attached to the frame by the VHB G23F tape.
For this study, steps 2 - 4 listed above were simulated in the finite element analysis.
Figure 2. Illustration of the bonding process simulated in this study.
Finite Element Models and Analysis 1. The Glazing Panel Model Figs. 2 and 3 illustrate the warped glass panel with a single arch investigated here. The arch is a shallow circular arch. The warpage is defined by the ratio of the arch height variation over a unit
edge length of the panel. A total of six warpage scenarios were studied with warpage ranging from 0.13% to 0.33% as listed in Fig. 3. All the arch heights are within the allowable range of ASTM C 1048. The dimensions of the panel assembly are shown in Fig. 4.
Case Warpage Max gap, d (mm)
1 16 mil / foot = 0.13% 3.25
2 24 mil / foot = 0.20% 4.88
3 28 mil / foot = 0.23% 5.69
4 32 mil / foot = 0.27% 6.51
5 36 mil / foot = 0.30% 7.32
6 40 mil / foot = 0.33% 8.13
Figure 3. Illustration of the warped glass, and the gap between the glass panel and the tape. The dimensions of the glass panel and the tape are specified in Fig. 3.
Figure 4. Illustration of the glass panel and the tape.
2. Finite Element Analysis A 3-dimensional finite element analysis was performed using ABAQUS simulation software to investigate the deformation of the VHB G23F tape and the glass panel deformation during assembly. The metal glazing frame was assumed to be rigid, and its effect was represented by a fixed boundary condition on the side of the tape bonded to the frame, allowing the omission of the frame from the finite element model. Only the tape and the warped glass illustrated in Fig. 4 are simulated in the finite element analysis. Two bonding pressure application methods were modeled:
Bonding by pressing a roller with a force of 222 N (50 lb) traveling at a speed of 0.04 m/s (0.13 ft/sec).
Bonding by applying a pressure of 425 kPa (62 psi) over the bond area. This pressure is referred to as edge pressure in this paper.
The uniform bonding pressure over the edges of the...